Microwave Sintering of Aluminum-ZrB Composite: Sintering of Aluminum-ZrB 2 Composite: Focusing on...
Embed Size (px)
Transcript of Microwave Sintering of Aluminum-ZrB Composite: Sintering of Aluminum-ZrB 2 Composite: Focusing on...
DOI: http://dx.doi.org/10.1590/1980-5373-MR-2015-0799Materials Research. 2016; 19(4): 765-769 2016
Microwave Sintering of Aluminum-ZrB2 Composite: Focusing on Microstructure and Mechanical Properties
Ehsan Ghasalia,b*, Rahim Yazdani-radb, Ali Rahbarib, Touradj Ebadzadehb
aSama Technical and Vocational Training College, Islamic Azad University, Eslamshahr, Tehran, IranbCeramic Department, Materials and Energy Research Center, Tehran, Iran
Received: December 31, 2015; Revised: March 12, 2016; Accepted: April 27, 2016
Microwave assisted rapid sintering was carried out to fabricate aluminum-ZrB2 metal matrix composites containing 1 wt% cobalt and 10, 15 and 20 wt% ZrB2 as the reinforcements at temperatures of 600, 700 and 800C. The results showed that the highest values of density and bending strength (97% of theoretical density and 240 MPa, respectively) were obtained in a composite containing 15 wt% ZrB2 and 1 wt% Co sintered at 600C. Furthermore, the optimum values of compressive strength and hardness (350 MPa and 63 Vickers, respectively) were measured for a composite containing 20 wt% ZrB2 sintered at 600C. At all sintering temperatures, XRD analysis revealed ZrB2 and aluminum as the only crystalline phases. Microstructure investigations demonstrated a homogeneous distribution of ZrB2 particles in the aluminum matrix.
Keywords: Aluminum, Zirconium diboride, Microwave sintering, Metal matrix composites
1. IntroductionAluminum (Al) metal matrix composites (AMC) have
many applications in the aerospace and car industries and military applications due to their high specific modulus, high strength to weight ratio and toughness1-3. Generally, the casting, extrusion and forging routes, and powder metallurgy (PM) process have been used to produce AMC4,5. Compared with traditional methods, PM is believed to be a more appropriate process to fabricate near net shape products6. In addition, the interaction between matrix and reinforcements can be avoided because of lower processing temperatures usually associated with PM methods7. Compared with casting process, PM provides a more uniform distribution of reinforcement materials within the matrix8. However, the conventional PM processing of composites often needs long sintering time, which results in grain coarsening and poor performance of mechanical properties9.
Microwave sintering presents distinct advantages such as high energy efficiency, enhanced densification and also smaller grain size due to the faster heating rate at lower sintering temperatures10. Microwave sintering provides a uniform volumetric heating as well as smaller pores in the sintered compacts, which improves the microstructure and mechanical properties11-13.
SiC and Al2O3 particles are the most commonly used materials for reinforcement of Al alloys. Furthermore, there has been growing interest of using ZrB2 as reinforcement due to its high melting point, high electrical and thermal conductivity and chemical inertness14-16. In the recent years, there has been much research into various aspects of Al-ZrB2 composites produced mainly by casting route and PM method17,18. The limited research has been conducted on the effect of second metallic phase as a binder or coherent phase between aluminum and reinforcement19. Some researchers investigated the effect of Cu additive as
a coating of reinforcement particles on different aluminum matrix composites20. However, to the best of the authors knowledge, there have been limited reports of the effect of Co additive on the final properties of Al-ZrB2 composites
21,22. In the present work, an attempt has been made to
investigate the effect of microwave sintering parameters and variable amounts of ZrB2 on microstructure and mechanical properties of PM green compacts. Additionally, the properties of Al-ZrB2 composite with and without 1 wt% Co have been investigated.
2. Experimental proceduresZrB2 (99.5% purity, 10 m average particle size) and
aluminum (MERCK Art. no. 1056 aluminum powder,
Ghasali et al. Materials Research766
the increase of sintering temperature. This is because of two diverse effects; the relative density increases as a result of high atomic diffusion and decreases due to the agglomeration of ZrB2 particles during sintering process. Because of high melting point of ZrB2, it can be expected that ZrB2 particles form aggregates with a random distribution in Al matrix, preventing complete densification14. Another possibility is the formation of alumina layer with a high melting point around Al particles and low tendency of these layers to make bonds with ZrB2 particles at sintering temperatures. It seems that the formation of some porosity and cracks within the composites matrix during cooling due to the thermal expansion mismatch between Al and ZrB2 particles can be prevented by adding Co particles.
3.3. Microstructural analysisThe backscattered electron images of Al-ZrB2 composites
are shown in figure 2. The dark and light regions correspond to Al and ZrB2 particles, respectively. SEM images in figure 2-a further reveal a uniform distribution of ZrB2 particles in Al matrix in C sample containing cobalt additive sintered at 600C. It also has a less porous structure (no cracks were observed), exhibiting good bonding between matrix and reinforcement particles.
Figure 2-b shows the scanning electron micrographs of A sample (without cobalt additive) sintered at 600C. Microcracks can be seen around ZrB2 particles attributed to the thermal expansion mismatch between Al and ZrB2 particles.
SEM micrographs of D composite sintered at 600C (Figure 2-c) show that the agglomeration of ZrB2 particles increased due to increasing amount of reinforcement particles from 15 to 20 wt%.
Figure 3 shows the SEM micrographs and EDS analysis of Al-15wt%ZrB2-1wt%Co composite sintered at 600C. EDS1 point (gray region) is rich in element Al, while EDS2 point (light region) is rich in element Zr, implying the existence of ZrB2 particles as the reinforcement in composite.
Figure 4 shows the fracture surface of C composite sintered at 600C. It can be observed that there are many fine dimples around 5-6 m in diameter accompanied by ZrB2 particles on the surface of this sample. The rupture mechanism of C composite is the ductile fracture of ZrB2 and its expanding in the substrate.
3.4. Bending strengthIn the case of sintering apart from bonding and porous-
free microstructure, the important factor affecting strength of sintered composite is the amount of ZrB2 particles presented in the matrix. On the other hand, increasing amounts of reinforcements can be caused the agglomeration of particles, destroying the mechanical properties of composites. The maximum bending strength value was measured for C composite containing 15 wt % ZrB2 and 1wt% Co sintered at 600C. The presence of ZrB2 particles in Al matrix could impede the movement of dislocations since these particles are stronger than Al particles. As it was considered in previous section (Figure 2-c), the agglomeration of reinforcement particles in Al-20 wt% ZrB2-1wt% Co composite could form some porosity between agglomerates, acting as crack propagation centers. The degree of strengthening produced
Table 1: Different batch compositions.
Batch Al (wt %) ZrB2 (wt %) Co (wt %)
A 90 10 0
B 89 10 1
C 84 15 1
D 79 20 1
and 3 samples, respectively. X-ray diffraction (XRD, Philips X Pert System) analyses were performed to identify the phases present in the Al-ZrB2 composites. Vickers microhardness values of the sintered samples were determined using a MKV-h21 Microhardness Tester under a load of 1kgf for 15 s. At least ten successive indentations were performed for each sample. Microstructural investigations of sintered samples were carried out using a SEM (Stereoscan 360, Leica Cambridge).
3. Results and discussion
3.1. XRD analysisFigure 1 shows the XRD patterns of D series samples
(table 1) sintered at 600, 700 and 800C. The identified phases of Al and ZrB2 are similar for all composites and no additional phases are found.
Figure 1: XRD patterns of composites containing 20 wt% ZrB2 sintered at (a) 600 C, 700C and 800 C.
3.2. DensificationSince in the precision of XRD analysis only Al and
ZrB2 phases were detected (Figure 1), therefore, the relative density of composites were measured by the rule of mixtures and the results are shown in Table 2. The variation of the measured densities was limited to 1 % of the average value. As Table 2 further reveals, the relative densities of B, C and D composites are nearly the same compared to A composite which is much less. It seems that the presence of Co additive in B, C and D composites caused an increase of density. The maximum relative density of 96.90.3 % was calculated for C composite sintered at 600 C.
As Table 2 represents, there is no significant change in the measured density of Al-ZrB2 composites containing Co with
Microwave Sintering of Aluminum-ZrB2 Composite: Focusing on Microstructure and Mechanical Properties 767
Table 2: Relative density of composites sintered at different temperatures.
Al-20wt%ZrB2-1wt%Co Al-15wt%ZrB2-1wt%Co Al-10wt%ZrB2-1wt%Co Al-10wt%ZrB2 sample
3.06 2.96 2.88 2.85
800 700 600 800 700 600 800 700 600 800 700 600
Teoretical density (gr/cm3)
Sintering temperature (C)
Measured density (gr/cm3)